4 Semiconductor Manufacturing Process Fundamental Processing Steps1.Silicon Manufacturinga) Czochralski method.b) Wafer Manufacturingc) Crystal structure2.Photolithographya) Photoresistsb) Photomask and Reticlesc) Patterning
5 Semiconductor Manufacturing Process (cont) 3.Oxide Growth & Removala) Oxide Growth & Depositionb) Oxide Removalc) Other effectsd) Local Oxidation4. Diffusion & Ion Implantationa) Diffusionb) Other effectsc) Ion Implantation
6 Silicon Manufacturing Crystal Growth and Wafer Manufacturing
7 FABRICATING SILICON Quartz, or Silica, Consists of Silicon Dioxide Sand Contains Many Tiny Grains of QuartzSilicon Can be Artificially Produced by Combining Silica and Carbon in Electric FurniceGives Polycrystalline Silicon (multitude of crystals)Practical Integrated Circuits Can Only be Fabricated from Single-Crystal Material
8 CRYSTAL GROWTHCzochralski Process is a Technique in Making Single-Crystal SiliconA Solid Seed Crystal is Rotated and Slowly Extracted from a Pool of Molten SiRequires Careful Control to Give Crystals Desired Purity and Dimensions
9 CYLINDER OF MONOCRYSTALLINE The Silicon Cylinder is Known as an IngotTypical Ingot is About 1 or 2 Meters in LengthCan be Sliced into Hundreds of Smaller Circular Pieces Called WafersEach Wafer Yields Hundreds or Thousands of Integrated Circuits
10 WAFER MANUFACTURINGThe Silicon Crystal is Sliced by Using a Diamond-Tipped Saw into Thin WafersSorted by ThicknessDamaged Wafers Removed During LappingEtch Wafers in Chemical to Remove any Remaining Crystal DamagePolishing Smoothes Uneven Surface Left by Sawing Process
11 THE CRYSTAL STRUCTURE OF SILICON A Unit Cell Has 18 Silicons AtomsWeak Bonding Along Cleavage PlanesWafer Splits into 4 or 6 Wedge-Shaped FragmentsMiller Indices is Used to Assign to Each Possible Plane Passing Through the Crystal Lattice
13 PhotolithographyPhotolithography is a technique that is used to define the shape of micro-machined structures on a wafer.
14 Photolithography Photoresist The first step in the photolithography process is to develop a mask, which will be typically be a chromium pattern on a glass plate.Next, the wafer is then coated with a polymer which is sensitive to ultraviolet light called a photoresist.Afterward, the photoresist is then developed which transfers the pattern on the mask to the photoresist layer.
15 Photolithography Photoresist There are two basic types of Photoresists Positive and Negative.Positive resists.Positive resists decomposes ultraviolet light. The resist is exposed with UV light wherever the underlying material is to be removed. In these resists, exposure to the UV light changes the chemical structure of the resist so that it becomes more soluble in the developer. The exposed resist is then washed away by the developer solution, leaving windows of the bare underlying material. The mask, therefore, contains an exact copy of the pattern which is to remain on the wafer.
16 Photolithography Photoresist Negative resistsExposure to the UV light causes the negative resist to become polymerized, and more difficult to dissolve. Therefore, the negative resist remains on the surface wherever it is exposed, and the developer solution removes only the unexposed portions. Masks used for negative photoresists, therefore, contain the inverse (or photographic "negative") of the pattern to be transferred.
17 Photolithography Model Figure 1a shows a thin film of some material (eg, silicon dioxide) on a substrate of some other material (eg, a silicon wafer).Photoresist layer (Figure 1b )Ultraviolet light is then shone through the mask onto the photoresist (figure 1c).
18 Photolithography Model (cont) The photoresist is then developed which transfers the pattern on the mask to the photoresist layer (figure 1d).A chemical (or some other method) is then used to remove the oxide where it is exposed through the openings in the resist (figure 1e).Finally the resist is removed leaving the patterned oxide (figure 1f).
19 Photolithography Photomasks and Reticles This is a square glass plate with a patterned emulsion of metal film on one side. The mask is aligned with the wafer, so that the pattern can be transferred onto the wafer surface. Each mask after the first one must be aligned to the previous pattern.
20 Photolithography Photomasks and Reticles When a image on the photomask is projected several time side by side onto the wafer, this is known as stepping and the photomask is called a reticle.An common reticle is the 5XThe patterns on the 5X reticle are reduced 5 times when projected onto the wafer. This means the dies on the photomask are 5 times larger than they are on the final product. There are other kinds of reduction reticles (2X, 4X, and 10X), but the 5X is the most commonly used. Reduction reticles are used on a variety of steppers, the most common being ASM, Canon, Nikon, and GCA.
21 Photolithography Photomasks and Reticles Examples of 5X Reticles:
22 Photolithography Photomasks and Reticles Once the mask has been accurately aligned with the pattern on the wafer's surface, the photoresist is exposed through the pattern on the mask with a high intensity ultraviolet light. There are three primary exposure methods: contact, proximity, and projection.
23 Photolithography Patterning The last stage of Photolithography is a process called ashing. This process has the exposed wafers sprayed with a mixture of organic solvents that dissolves portions of the photoresist .Conventional methods of ashing require an oxygen-plasma ash, often in combination with halogen gases, to penetrate the crust and remove the photoresist. Usually, the plasma ashing process also requires a follow-up cleaning with wet-chemicals and acids to remove the residues and non-volatile contaminants that remain after ashing. Despite this treatment, it is not unusual to repeat the "ash plus wet-clean" cycle in order to completely remove all photoresist and residues.
25 SiO2 growth is a key process step in manufacturing all Si devices - Thick ( 1µm) oxides are used for field oxides (isolate devices from one another )- Thin gate oxides (100 Å) control MOS devices - Sacrificial layers are grown and removed to clean up surfacesThe stability and ease of formation of SiO2 was one of the reasons that Si replaced Ge as the semiconductor of choice.
26 The simplest method of producing an oxide layer consists of heating a silicon wafer in an oxidizing atmosphere.
27 Dry oxide - Pure dry oxygen is employed Disadvantage- Dry oxide grows very slowly.Advantage- Oxide layers are very uniform.- Relatively few defects exist at the oxide-siliconinterface (These defects interfere with the properoperation of semiconductor devices)- It has especially low surface state charges and thus make ideal dielectrics for MOS transistors.
28 Wet oxide - In the same way as dry oxides, but steam is injected Disadvantage- Hydrogen atoms liberated by the decomposition of the water molecules produce imperfections that may degrade the oxide quality.Advantage- Wet oxide grows fast.- Useful to grow a thick layer of field oxide
29 Deposited OxidesOxide is frequently employed as an insulator between two layers of metalization. In such cases, some form of deposited oxide must be used rather than the grown oxides.Deposited oxides can be produced by various reactions between gaseous silicon compounds and gaseous oxidizers. Deposited oxides tend to possess low densities and large numbers of defect sites. Not suitable for use as gate dielectrics for MOS transistors but still acceptable for use as insulating layers between multiple conductor layers, or as protective overcoats.
30 Key Variables in Oxidation Temperature- reaction rate- solid state diffusionOxidizing species- wet oxidation is much faster than dry oxidationSurface cleanliness- metallic contamination can catalyze reaction- quality of oxide grown (interface states)
31 EtchingEtching is the process where unwanted areas of films are removed by either dissolving them in a wet chemical solution (Wet Etching) or by reacting them with gases in a plasma to form volatile products (Dry Etching).Resist protects areas which are to remain. In some cases a hard mask, usually patterned layers of SiO2 or Si3N4, are used when the etch selectivity to photoresist is low or the etching environment causes resist to delaminate.This is part of lithography - pattern transfer.
33 Wet Chemical Etching Wet etches: - are in general isotropic (not used to etch features less than ≈ 3 µm)- achieve high selectivities for most filmcombinations- capable of high throughputs- use comparably cheap equipment- can have resist adhesion problems- can etch just about anything
34 Example Wet Processes For SiO2 etching - HF + NH4F+H20 (buffered oxide etch or BOE)For Si3N4- Hot phosphoric acid: H3PO4 at 180 °C- need to use oxide hard maskSilicon- Nitric, HF, acetic acids- HNO3 + HF + CH3COOH + H2OAluminum- Acetic, nitric, phosphoric acids at °C- CH3COOH+HNO3+H3PO4
35 What is a plasma (glow discharge)? A plasma is a partially ionized gas made up of equal parts positively and negatively charged particles.Plasmas are generated by flowing gases through an electric or magnetic field.These fields remove electrons from some of the gas molecules. The liberated electrons are accelerated, or energized, by the fields.The energetic electrons slam into other gas molecules, liberating more electrons, which are accelerated and liberate more electrons from gas molecules, thus sustaining the plasma.
38 Dry or Plasma EtchingCombination of chemical and physical etching – Reactive Ion Etching (RIE)Directional etching due to ion assistance.In RIE processes the wafers sit on the powered electrode. This placement sets up a negative bias on the wafer which accelerates positively charge ions toward the surface. These ions enhance the chemical etching mechanisms and allow anisotropic etching.Wet etches are simpler, but dry etches provide better line width control since it is anisotropic.
39 Other Effects of Oxide Growth and Removal Oxide StepThe differences in oxide thickness and in the depths of the silicon surfaces combine to produce a characteristic surface discontinuityThe growth of a thermal oxide affects the doping levels in the underlying siliconThe doping of silicon affects the rate of oxide growth
40 Local Oxidation of Silicon (LOCOS) LOCOS: localized oxidation of silicon using silicon nitride as a mask against thermal oxidation.A technique called local oxidation of silicon (LOCOS) allows the selective growth thick oxide layersCMOS and BiCMOS processes employ LOCOS to grow a thick field oxide over electrically inactive regions of the wafer
41 Silicon Manufacturing Diffusion and Ion Implantation
42 WN-Junction Fabrication (Earliest method) Process:Opposite polarity doping atoms are added to molten silicon during the Czochralski process to create in-grown junctions in the ingot.Repeated counterdopings can produce multiple junctions within the crystal.DisadvantagesInability to produce differently doped areas in different parts of the wafer.The thickness and planarity of grown junctions are difficult to control.Repeated counterdopings degrade the electrical properties of the silicon.
43 The Planar Process Advantages: The planar process does not require multiple counterdopings of the silicon ingot.This process allows more precise control of junction depths and dopant distributions.
44 Methods of planar process DiffusionA uniformly doped ingot is sliced into wafers.An oxide film is then grown on the wafers.The film is patterned and etched using photolithography exposing specific sections of the silicon.The wafers are then spun with an opposite polarity doping source adhering only to the exposed areas.The wafers are then heated in a furnace ( deg.C) to drive the doping atoms into the silicon.Ion ImplantationA particle accelerator is used to accelerate a doping atom so that it can penetrate a silicon crystal to a depth of several micronsLattice damage to the crystal is then repaired by heating the wafer at a moderate temperature for a few minutes. This process is called annealing.
46 Comparison of Diffusion and Ion Implantation Diffusion is a cheaper and more simplistic method, but can only be performed from the surface of the wafers. Dopants also diffuse unevenly, and interact with each other altering the diffusion rate.Ion implantation is more expensive and complex. It does not require high temperatures and also allows for greater control of dopant concentration and profile. It is an anisotropic process and therefore does not spread the dopant implant as much as diffusion. This aids in the manufacture of self-aligned structures which greatly improve the performance of MOS transistors.
47 ReferencesThe Art of Analog Layout by Alan Hastings 2001 Prentice-HallSemiconductor Devices by Mauro Zambuto 1989 McGraw-HillSemiconductor Manufacturing Technology by Quirk and Serda 2001 Prentice-Hall